# Electronic Supplementary Material (ESI) for Physical Chemistry Chemical Physics.
# This journal is © the Owner Societies 2014

#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_is_high

_audit_creation_method           SHELXL-97
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_formula_moiety         'F4 Mg Sr'
_chemical_formula_sum            'F4 Mg Sr'
_chemical_melting_point          ?

_exptl_crystal_description       prism
_exptl_crystal_colour            colorless

_diffrn_ambient_temperature      473(2)
_chemical_formula_weight         187.93

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sr Sr -1.5307 3.2498 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_H-M   'C m c 21'
_symmetry_space_group_name_Hall  'C 2c -2'
_symmetry_int_tables_number      36
_chemical_absolute_configuration ?

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, z'
'x, -y, z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z+1/2'

_cell_length_a                   3.937(3)
_cell_length_b                   14.488(9)
_cell_length_c                   5.638(4)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     321.6(4)
_cell_formula_units_Z            4
_cell_measurement_temperature    473(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      ?
_cell_measurement_theta_max      ?
_exptl_crystal_size_max          0.19
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.11
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.882
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             344
_exptl_absorpt_coefficient_mu    16.880

_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.1435
_exptl_absorpt_correction_T_max  0.2653
_exptl_absorpt_process_details   'Bruker SADABS'

_exptl_special_details           
; 
 ? 
;


_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker Nonius X8Apex CCD area-detector'
_diffrn_measurement_method       'φ scans'
_diffrn_detector_area_resol_mean 25
_diffrn_standards_number         0
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        0
_diffrn_reflns_number            914
_diffrn_reflns_av_R_equivalents  0.0865
_diffrn_reflns_av_sigmaI/netI    0.0805
_diffrn_reflns_limit_h_min       -4
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_theta_min         2.81
_diffrn_reflns_theta_max         25.55
_reflns_number_total             347
_reflns_number_gt                339
_reflns_threshold_expression     >2σ(I)


_computing_data_collection       'Bruker APEX2'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'Bruker SHELXTL'
_computing_structure_refinement  'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0842P)²+0.0812P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   ?
_refine_ls_hydrogen_treatment    noref
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.0232(12)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.03(3)
_refine_ls_number_reflns         347
_refine_ls_number_parameters     38
_refine_ls_number_restraints     7
_refine_ls_R_factor_all          0.0522
_refine_ls_R_factor_gt           0.0520
_refine_ls_wR_factor_ref         0.1283
_refine_ls_wR_factor_gt          0.1280
_refine_ls_goodness_of_fit_ref   1.104
_refine_ls_restrained_S_all      1.116
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Sr1 Sr 0.0000 0.34183(8) 0.04618(13) 0.0216(7) Uani 1 2 d S . .
Mg1 Mg 0.5000 0.4165(3) 0.5948(7) 0.0134(12) Uani 1 2 d S . .
F1 F 0.5000 0.3398(4) 0.313(2) 0.020(2) Uani 1 2 d S . .
F2 F 0.5000 0.5327(5) 0.4291(17) 0.027(2) Uani 1 2 d SU . .
F3 F 0.5000 0.2999(5) 0.7869(18) 0.0173(19) Uani 1 2 d S . .
F4 F 0.0000 0.4157(8) 0.613(2) 0.037(3) Uani 1 2 d S . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sr1 F3 2.462(8) 6_554 ?
Sr1 F1 2.478(7) . ?
Sr1 F1 2.478(7) 1_455 ?
Sr1 F3 2.526(6) 1_454 ?
Sr1 F3 2.526(6) 1_554 ?
Sr1 F4 2.669(11) 1_554 ?
Sr1 F2 2.760(5) 2_664 ?
Sr1 F2 2.760(5) 2_564 ?
Sr1 F1 2.941(7) 6_554 ?
Sr1 Mg1 3.395(4) 1_454 ?
Sr1 Mg1 3.395(4) 1_554 ?
Sr1 Mg1 3.753(5) 6_554 ?
Mg1 F2 1.925(9) . ?
Mg1 F1 1.939(12) . ?
Mg1 F4 1.9710(15) 1_655 ?
Mg1 F4 1.9710(15) . ?
Mg1 F3 2.007(9) . ?
Mg1 F2 2.023(10) 2_665 ?
Mg1 Sr1 3.395(4) 1_656 ?
Mg1 Sr1 3.395(4) 1_556 ?
Mg1 Sr1 3.753(5) 6 ?
Mg1 Sr1 3.823(4) 1_655 ?
Mg1 Sr1 4.026(4) 2_665 ?
F1 Sr1 2.478(7) 1_655 ?
F1 Sr1 2.941(7) 6 ?
F2 Mg1 2.023(10) 2_664 ?
F2 Sr1 2.760(5) 2_665 ?
F2 Sr1 2.760(5) 2_565 ?
F3 Sr1 2.462(8) 6 ?
F3 Sr1 2.526(6) 1_656 ?
F3 Sr1 2.526(6) 1_556 ?
F4 Mg1 1.9710(15) 1_455 ?
F4 Sr1 2.669(11) 1_556 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F3 Sr1 F1 69.83(19) 6_554 . ?
F3 Sr1 F1 69.83(19) 6_554 1_455 ?
F1 Sr1 F1 105.2(4) . 1_455 ?
F3 Sr1 F3 96.81(10) 6_554 1_454 ?
F1 Sr1 F3 165.4(2) . 1_454 ?
F1 Sr1 F3 74.3(3) 1_455 1_454 ?
F3 Sr1 F3 96.81(10) 6_554 1_554 ?
F1 Sr1 F3 74.3(3) . 1_554 ?
F1 Sr1 F3 165.4(2) 1_455 1_554 ?
F3 Sr1 F3 102.4(4) 1_454 1_554 ?
F3 Sr1 F4 147.1(3) 6_554 1_554 ?
F1 Sr1 F4 124.1(2) . 1_554 ?
F1 Sr1 F4 124.1(2) 1_455 1_554 ?
F3 Sr1 F4 64.3(2) 1_454 1_554 ?
F3 Sr1 F4 64.3(2) 1_554 1_554 ?
F3 Sr1 F2 132.96(14) 6_554 2_664 ?
F1 Sr1 F2 65.6(2) . 2_664 ?
F1 Sr1 F2 136.0(3) 1_455 2_664 ?
F3 Sr1 F2 125.2(3) 1_454 2_664 ?
F3 Sr1 F2 57.6(2) 1_554 2_664 ?
F4 Sr1 F2 61.1(3) 1_554 2_664 ?
F3 Sr1 F2 132.96(14) 6_554 2_564 ?
F1 Sr1 F2 136.0(3) . 2_564 ?
F1 Sr1 F2 65.6(2) 1_455 2_564 ?
F3 Sr1 F2 57.6(2) 1_454 2_564 ?
F3 Sr1 F2 125.2(3) 1_554 2_564 ?
F4 Sr1 F2 61.1(3) 1_554 2_564 ?
F2 Sr1 F2 91.0(2) 2_664 2_564 ?
F3 Sr1 F1 60.0(3) 6_554 6_554 ?
F1 Sr1 F1 105.11(11) . 6_554 ?
F1 Sr1 F1 105.11(11) 1_455 6_554 ?
F3 Sr1 F1 61.73(19) 1_454 6_554 ?
F3 Sr1 F1 61.73(19) 1_554 6_554 ?
F4 Sr1 F1 87.1(3) 1_554 6_554 ?
F2 Sr1 F1 118.8(2) 2_664 6_554 ?
F2 Sr1 F1 118.8(2) 2_564 6_554 ?
F3 Sr1 Mg1 132.80(16) 6_554 1_454 ?
F1 Sr1 Mg1 156.89(18) . 1_454 ?
F1 Sr1 Mg1 89.9(2) 1_455 1_454 ?
F3 Sr1 Mg1 35.99(18) 1_454 1_454 ?
F3 Sr1 Mg1 95.4(2) 1_554 1_454 ?
F4 Sr1 Mg1 35.45(5) 1_554 1_454 ?
F2 Sr1 Mg1 91.39(17) 2_664 1_454 ?
F2 Sr1 Mg1 36.6(2) 2_564 1_454 ?
F1 Sr1 Mg1 87.15(19) 6_554 1_454 ?
F3 Sr1 Mg1 132.80(16) 6_554 1_554 ?
F1 Sr1 Mg1 89.9(2) . 1_554 ?
F1 Sr1 Mg1 156.89(18) 1_455 1_554 ?
F3 Sr1 Mg1 95.4(2) 1_454 1_554 ?
F3 Sr1 Mg1 35.99(18) 1_554 1_554 ?
F4 Sr1 Mg1 35.45(5) 1_554 1_554 ?
F2 Sr1 Mg1 36.6(2) 2_664 1_554 ?
F2 Sr1 Mg1 91.39(17) 2_564 1_554 ?
F1 Sr1 Mg1 87.15(19) 6_554 1_554 ?
Mg1 Sr1 Mg1 70.88(9) 1_454 1_554 ?
F3 Sr1 Mg1 29.3(2) 6_554 6_554 ?
F1 Sr1 Mg1 86.78(16) . 6_554 ?
F1 Sr1 Mg1 86.78(16) 1_455 6_554 ?
F3 Sr1 Mg1 78.61(17) 1_454 6_554 ?
F3 Sr1 Mg1 78.61(17) 1_554 6_554 ?
F4 Sr1 Mg1 117.8(3) 1_554 6_554 ?
F2 Sr1 Mg1 132.41(12) 2_664 6_554 ?
F2 Sr1 Mg1 132.41(12) 2_564 6_554 ?
F1 Sr1 Mg1 30.7(2) 6_554 6_554 ?
Mg1 Sr1 Mg1 111.88(9) 1_454 6_554 ?
Mg1 Sr1 Mg1 111.88(9) 1_554 6_554 ?
F2 Mg1 F1 96.0(4) . . ?
F2 Mg1 F4 91.7(3) . 1_655 ?
F1 Mg1 F4 92.2(4) . 1_655 ?
F2 Mg1 F4 91.7(3) . . ?
F1 Mg1 F4 92.2(4) . . ?
F4 Mg1 F4 174.1(6) 1_655 . ?
F2 Mg1 F3 176.4(4) . . ?
F1 Mg1 F3 87.7(4) . . ?
F4 Mg1 F3 88.1(3) 1_655 . ?
F4 Mg1 F3 88.1(3) . . ?
F2 Mg1 F2 97.7(2) . 2_665 ?
F1 Mg1 F2 166.3(4) . 2_665 ?
F4 Mg1 F2 87.4(4) 1_655 2_665 ?
F4 Mg1 F2 87.4(4) . 2_665 ?
F3 Mg1 F2 78.6(4) . 2_665 ?
F2 Mg1 Sr1 130.0(2) . 1_656 ?
F1 Mg1 Sr1 115.6(2) . 1_656 ?
F4 Mg1 Sr1 51.7(3) 1_655 1_656 ?
F4 Mg1 Sr1 122.6(3) . 1_656 ?
F3 Mg1 Sr1 47.7(2) . 1_656 ?
F2 Mg1 Sr1 54.37(17) 2_665 1_656 ?
F2 Mg1 Sr1 130.0(2) . 1_556 ?
F1 Mg1 Sr1 115.6(2) . 1_556 ?
F4 Mg1 Sr1 122.6(3) 1_655 1_556 ?
F4 Mg1 Sr1 51.7(3) . 1_556 ?
F3 Mg1 Sr1 47.7(2) . 1_556 ?
F2 Mg1 Sr1 54.37(17) 2_665 1_556 ?
Sr1 Mg1 Sr1 70.88(9) 1_656 1_556 ?
F2 Mg1 Sr1 146.8(3) . 6 ?
F1 Mg1 Sr1 50.8(2) . 6 ?
F4 Mg1 Sr1 89.9(4) 1_655 6 ?
F4 Mg1 Sr1 89.9(4) . 6 ?
F3 Mg1 Sr1 36.9(3) . 6 ?
F2 Mg1 Sr1 115.5(3) 2_665 6 ?
Sr1 Mg1 Sr1 74.73(8) 1_656 6 ?
Sr1 Mg1 Sr1 74.73(8) 1_556 6 ?
F2 Mg1 Sr1 81.7(3) . . ?
F1 Mg1 Sr1 34.39(11) . . ?
F4 Mg1 Sr1 123.6(4) 1_655 . ?
F4 Mg1 Sr1 61.6(3) . . ?
F3 Mg1 Sr1 101.4(3) . . ?
F2 Mg1 Sr1 148.95(4) 2_665 . ?
Sr1 Mg1 Sr1 144.58(12) 1_656 . ?
Sr1 Mg1 Sr1 102.57(7) 1_556 . ?
Sr1 Mg1 Sr1 70.04(7) 6 . ?
F2 Mg1 Sr1 81.7(3) . 1_655 ?
F1 Mg1 Sr1 34.39(11) . 1_655 ?
F4 Mg1 Sr1 61.6(3) 1_655 1_655 ?
F4 Mg1 Sr1 123.6(4) . 1_655 ?
F3 Mg1 Sr1 101.4(3) . 1_655 ?
F2 Mg1 Sr1 148.95(4) 2_665 1_655 ?
Sr1 Mg1 Sr1 102.57(7) 1_656 1_655 ?
Sr1 Mg1 Sr1 144.58(12) 1_556 1_655 ?
Sr1 Mg1 Sr1 70.04(7) 6 1_655 ?
Sr1 Mg1 Sr1 61.99(8) . 1_655 ?
F2 Mg1 Sr1 37.50(17) . 2_665 ?
F1 Mg1 Sr1 116.3(2) . 2_665 ?
F4 Mg1 Sr1 61.4(4) 1_655 2_665 ?
F4 Mg1 Sr1 119.8(4) . 2_665 ?
F3 Mg1 Sr1 140.2(2) . 2_665 ?
F2 Mg1 Sr1 75.4(2) 2_665 2_665 ?
Sr1 Mg1 Sr1 92.56(7) 1_656 2_665 ?
Sr1 Mg1 Sr1 127.72(11) 1_556 2_665 ?
Sr1 Mg1 Sr1 149.58(5) 6 2_665 ?
Sr1 Mg1 Sr1 116.30(10) . 2_665 ?
Sr1 Mg1 Sr1 86.53(7) 1_655 2_665 ?
Mg1 F1 Sr1 119.4(2) . . ?
Mg1 F1 Sr1 119.4(2) . 1_655 ?
Sr1 F1 Sr1 105.2(4) . 1_655 ?
Mg1 F1 Sr1 98.5(4) . 6 ?
Sr1 F1 Sr1 106.38(18) . 6 ?
Sr1 F1 Sr1 106.38(18) 1_655 6 ?
Mg1 F2 Mg1 140.3(5) . 2_664 ?
Mg1 F2 Sr1 117.4(3) . 2_665 ?
Mg1 F2 Sr1 89.0(2) 2_664 2_665 ?
Mg1 F2 Sr1 117.4(3) . 2_565 ?
Mg1 F2 Sr1 89.0(2) 2_664 2_565 ?
Sr1 F2 Sr1 91.0(2) 2_665 2_565 ?
Mg1 F3 Sr1 113.9(5) . 6 ?
Mg1 F3 Sr1 96.3(2) . 1_656 ?
Sr1 F3 Sr1 121.31(17) 6 1_656 ?
Mg1 F3 Sr1 96.3(2) . 1_556 ?
Sr1 F3 Sr1 121.31(17) 6 1_556 ?
Sr1 F3 Sr1 102.4(4) 1_656 1_556 ?
Mg1 F4 Mg1 174.1(6) 1_455 . ?
Mg1 F4 Sr1 92.8(3) 1_455 1_556 ?
Mg1 F4 Sr1 92.8(3) . 1_556 ?

_diffrn_measured_fraction_theta_max 0.995
_diffrn_reflns_theta_full        25.50
_diffrn_measured_fraction_theta_full 0.995
_refine_diff_density_max         1.588
_refine_diff_density_min         -1.141
_refine_diff_density_rms         0.325
_database_code_depnum_ccdc_archive 'CCDC 1029321'
#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_is_low

_audit_creation_method           SHELXL-97
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_formula_moiety         'F4 Mg Sr'
_chemical_formula_sum            'F4 Mg Sr'
_chemical_melting_point          ?

_exptl_crystal_description       prism
_exptl_crystal_colour            colorless

_diffrn_ambient_temperature      150(2)
_chemical_formula_weight         187.93

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sr Sr -1.5307 3.2498 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'P 21'
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_int_tables_number      4
_chemical_absolute_configuration ad

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z'

_cell_length_a                   7.4736(5)
_cell_length_b                   16.8835(12)
_cell_length_c                   7.8010(5)
_cell_angle_alpha                90.00
_cell_angle_beta                 105.030(2)
_cell_angle_gamma                90.00
_cell_volume                     950.66(11)
_cell_formula_units_Z            12
_cell_measurement_temperature    150(2)
_cell_measurement_reflns_used    4496
_cell_measurement_theta_min      2.82
_cell_measurement_theta_max      36.30
_exptl_crystal_size_max          0.19
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.11
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.939
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1032
_exptl_absorpt_coefficient_mu    17.130

_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.1410
_exptl_absorpt_correction_T_max  0.2615
_exptl_absorpt_process_details   'SADABS (Bruker, 2004)'

_exptl_special_details           
; 
 ? 
;


_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker Nonius X8Apex CCD area-detector'
_diffrn_measurement_method       'φ scans'
_diffrn_detector_area_resol_mean 25
_diffrn_standards_number         0
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        0
_diffrn_reflns_number            11895
_diffrn_reflns_av_R_equivalents  0.0322
_diffrn_reflns_av_sigmaI/netI    0.0670
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_theta_min         2.41
_diffrn_reflns_theta_max         28.28
_reflns_number_total             4694
_reflns_number_gt                4017
_reflns_threshold_expression     >2σ(I)


_computing_data_collection       'APEX2 (Bruker, 2004)'
_computing_cell_refinement       'SAINT (Bruker, 2004)'
_computing_data_reduction        'SAINT (Bruker, 2004)'
_computing_structure_solution    'SHELXTL (Bruker, 2004)'
_computing_structure_refinement  'SHELXTL (Bruker, 2004)'
_computing_molecular_graphics    'SHELXTL (Bruker, 2004)'
_computing_publication_material  'SHELXTL (Bruker, 2004)'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   ?
_refine_ls_hydrogen_treatment    noref
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.008(5)
_refine_ls_number_reflns         4694
_refine_ls_number_parameters     325
_refine_ls_number_restraints     13
_refine_ls_R_factor_all          0.0321
_refine_ls_R_factor_gt           0.0235
_refine_ls_wR_factor_ref         0.0604
_refine_ls_wR_factor_gt          0.0560
_refine_ls_goodness_of_fit_ref   0.870
_refine_ls_restrained_S_all      0.867
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Sr1 Sr 0.65544(6) 0.19901(3) 0.16217(5) 0.00582(13) Uani 1 1 d . . .
Sr2 Sr 0.68190(8) 0.19041(3) 0.66833(6) 0.00587(9) Uani 1 1 d . . .
Sr3 Sr 0.34057(6) 0.36913(3) 0.33585(6) 0.00487(10) Uani 1 1 d . . .
Sr4 Sr 0.28834(10) 0.35176(3) 0.81853(7) 0.00678(11) Uani 1 1 d . . .
Sr5 Sr 0.66849(7) 0.53448(3) 0.16549(6) 0.00490(10) Uani 1 1 d . . .
Sr6 Sr 0.72761(6) 0.51632(3) 0.68180(6) 0.00543(12) Uani 1 1 d . . .
Mg1 Mg 0.16163(19) 0.17736(9) 0.04403(19) 0.0036(3) Uani 1 1 d . . .
Mg2 Mg 0.16787(19) 0.17643(9) 0.5398(2) 0.0037(3) Uani 1 1 d . . .
Mg3 Mg 0.8417(2) 0.34457(9) 0.4588(2) 0.0034(3) Uani 1 1 d . . .
Mg4 Mg 0.8376(2) 0.34510(9) 0.9621(2) 0.0038(3) Uani 1 1 d . . .
Mg5 Mg 0.17225(19) 0.51048(9) 0.0437(2) 0.0037(3) Uani 1 1 d . . .
Mg6 Mg 0.1719(2) 0.51245(9) 0.5435(2) 0.0034(3) Uani 1 1 d . . .
F1 F 0.0508(3) 0.07124(15) -0.0226(3) 0.0093(5) Uani 1 1 d U . .
F2 F 0.0696(3) 0.06443(14) 0.5487(3) 0.0075(5) Uani 1 1 d . . .
F3 F 0.3878(3) 0.11014(15) 0.1241(4) 0.0057(5) Uani 1 1 d . . .
F4 F 0.3985(3) 0.11080(15) 0.5741(4) 0.0047(5) Uani 1 1 d . . .
F5 F 0.7081(3) 0.11312(16) 0.4116(4) 0.0092(6) Uani 1 1 d . . .
F6 F 0.1186(3) 0.16313(15) 0.2810(3) 0.0093(5) Uani 1 1 d . . .
F7 F 0.2224(3) 0.17930(16) 0.8069(3) 0.0100(6) Uani 1 1 d . . .
F8 F 0.3279(3) 0.26997(16) 0.0978(3) 0.0065(5) Uani 1 1 d . . .
F9 F 0.3219(3) 0.27090(16) 0.5625(3) 0.0073(5) Uani 1 1 d . . .
F10 F 0.6116(3) 0.28067(16) 0.4125(3) 0.0055(5) Uani 1 1 d . . .
F11 F 0.5975(3) 0.28469(16) 0.8881(3) 0.0068(6) Uani 1 1 d . . .
F12 F 0.9500(3) 0.23901(15) 0.5338(3) 0.0101(5) Uani 1 1 d . . .
F13 F 0.9350(3) 0.23556(15) 0.9485(3) 0.0096(5) Uani 1 1 d . . .
F14 F 0.0779(3) 0.39740(15) 0.0418(3) 0.0075(5) Uani 1 1 d . . .
F15 F 0.0750(3) 0.40167(15) 0.4961(3) 0.0069(5) Uani 1 1 d . . .
F16 F 0.8372(4) 0.32380(16) 0.2098(3) 0.0093(5) Uani 1 1 d . . .
F17 F 0.8474(4) 0.36129(16) 0.7118(4) 0.0125(7) Uani 1 1 d . . .
F18 F 0.4006(3) 0.44493(16) 0.0743(3) 0.0071(5) Uani 1 1 d . . .
F19 F 0.4089(3) 0.44962(16) 0.6262(3) 0.0064(5) Uani 1 1 d . . .
F20 F 0.6730(3) 0.43610(16) 0.4041(4) 0.0065(6) Uani 1 1 d U . .
F21 F 0.7098(3) 0.44374(16) 0.9445(4) 0.0097(6) Uani 1 1 d . . .
F22 F 0.2204(4) 0.51001(16) 0.3046(3) 0.0094(6) Uani 1 1 d . . .
F23 F 0.1197(3) 0.49976(16) 0.7811(3) 0.0093(5) Uani 1 1 d . . .
F24 F 0.3378(3) 0.60451(16) 0.0725(4) 0.0079(6) Uani 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Sr1 F5 2.376(3) . ?
Sr1 F24 2.439(3) 2_645 ?
Sr1 F3 2.456(3) . ?
Sr1 F10 2.481(3) . ?
Sr1 F16 2.482(3) . ?
Sr1 F11 2.524(3) 1_554 ?
Sr1 F8 2.654(2) . ?
Sr1 F13 3.055(3) 1_554 ?
Sr1 F12 3.224(3) . ?
Sr1 Mg4 3.3875(16) 1_554 ?
Sr1 Mg3 3.4146(16) . ?
Sr1 Mg1 3.5832(14) . ?
Sr2 F5 2.440(3) . ?
Sr2 F4 2.455(2) . ?
Sr2 F10 2.457(3) . ?
Sr2 F24 2.523(3) 2_646 ?
Sr2 F11 2.536(3) . ?
Sr2 F13 2.606(2) . ?
Sr2 F12 2.623(2) . ?
Sr2 F9 2.935(3) . ?
Sr2 F17 3.123(3) . ?
Sr2 F22 3.127(3) 2_646 ?
Sr2 Mg3 3.4475(16) . ?
Sr2 Mg4 3.4705(16) . ?
Sr3 F9 2.454(3) . ?
Sr3 F10 2.462(3) . ?
Sr3 F8 2.484(3) . ?
Sr3 F22 2.532(3) . ?
Sr3 F18 2.545(3) . ?
Sr3 F19 2.577(3) . ?
Sr3 F14 2.647(2) . ?
Sr3 F20 2.655(3) . ?
Sr3 F15 2.663(2) . ?
Sr3 Mg5 3.3143(16) . ?
Sr3 Mg6 3.3359(16) . ?
Sr3 Mg3 3.6407(16) . ?
Sr4 F9 2.485(3) . ?
Sr4 F11 2.503(2) . ?
Sr4 F18 2.508(3) 1_556 ?
Sr4 F8 2.531(3) 1_556 ?
Sr4 F19 2.548(3) . ?
Sr4 F15 2.738(2) . ?
Sr4 F14 2.742(3) 1_556 ?
Sr4 F23 2.780(3) . ?
Sr4 F7 2.951(3) . ?
Sr4 F17 3.187(3) 1_455 ?
Sr4 Mg6 3.4281(16) . ?
Sr4 Mg5 3.4364(16) 1_556 ?
Sr5 F21 2.386(3) 1_554 ?
Sr5 F18 2.462(3) . ?
Sr5 F20 2.489(3) . ?
Sr5 F3 2.534(3) 2_655 ?
Sr5 F4 2.562(3) 2_656 ?
Sr5 F7 2.569(3) 2_656 ?
Sr5 F2 2.607(2) 2_656 ?
Sr5 F24 2.665(3) . ?
Sr5 F1 2.691(2) 2_655 ?
Sr5 Mg2 3.3264(16) 2_656 ?
Sr5 Mg1 3.3435(15) 2_655 ?
Sr5 Mg5 3.6047(15) . ?
Sr6 F21 2.421(3) . ?
Sr6 F3 2.495(3) 2_656 ?
Sr6 F20 2.497(3) . ?
Sr6 F4 2.538(3) 2_656 ?
Sr6 F19 2.568(2) . ?
Sr6 F6 2.716(3) 2_656 ?
Sr6 F17 2.757(3) . ?
Sr6 F2 2.758(3) 2_656 ?
Sr6 F23 2.844(2) 1_655 ?
Sr6 F1 2.896(3) 2_656 ?
Sr6 Mg2 3.4070(16) 2_656 ?
Sr6 Mg1 3.4256(16) 2_656 ?
Mg1 F13 1.933(3) 1_454 ?
Mg1 F6 1.972(3) . ?
Mg1 F8 1.973(3) . ?
Mg1 F1 1.986(3) . ?
Mg1 F3 1.997(3) . ?
Mg1 F7 2.016(3) 1_554 ?
Mg1 Sr5 3.3435(15) 2_645 ?
Mg1 Sr6 3.4256(16) 2_646 ?
Mg1 Mg4 3.673(2) 1_454 ?
Mg1 Sr4 3.6776(16) 1_554 ?
Mg2 F12 1.931(3) 1_455 ?
Mg2 F9 1.948(3) . ?
Mg2 F6 1.969(3) . ?
Mg2 F4 2.008(3) . ?
Mg2 F7 2.017(3) . ?
Mg2 F2 2.036(3) . ?
Mg2 Sr5 3.3264(16) 2_646 ?
Mg2 Sr6 3.4070(16) 2_646 ?
Mg2 Mg3 3.688(2) 1_455 ?
Mg2 Mg6 3.698(2) 2_546 ?
Mg3 F15 1.947(3) 1_655 ?
Mg3 F16 1.965(3) . ?
Mg3 F20 1.970(3) . ?
Mg3 F10 1.982(3) . ?
Mg3 F12 1.982(3) . ?
Mg3 F17 1.983(3) . ?
Mg3 Mg2 3.688(2) 1_655 ?
Mg3 Sr4 3.7650(17) 1_655 ?
Mg4 F21 1.907(3) . ?
Mg4 F14 1.953(3) 1_656 ?
Mg4 F16 1.966(3) 1_556 ?
Mg4 F17 1.992(3) . ?
Mg4 F13 2.000(3) . ?
Mg4 F11 2.014(3) . ?
Mg4 Sr1 3.3875(16) 1_556 ?
Mg4 Mg1 3.673(2) 1_656 ?
Mg4 Mg5 3.692(2) 1_656 ?
Mg4 Sr4 3.8172(16) 1_655 ?
Mg5 F1 1.928(3) 2 ?
Mg5 F22 1.973(3) . ?
Mg5 F24 1.989(3) . ?
Mg5 F23 1.992(3) 1_554 ?
Mg5 F18 1.996(3) . ?
Mg5 F14 2.034(3) . ?
Mg5 Sr4 3.4364(16) 1_554 ?
Mg5 Mg4 3.6919(19) 1_454 ?
Mg5 Sr6 3.7626(15) 1_454 ?
Mg5 Sr2 3.7674(17) 2_656 ?
Mg6 F5 1.911(3) 2_656 ?
Mg6 F2 1.967(3) 2_556 ?
Mg6 F22 1.989(3) . ?
Mg6 F23 2.002(3) . ?
Mg6 F15 2.005(3) . ?
Mg6 F19 2.021(3) . ?
Mg6 Mg2 3.698(2) 2_556 ?
Mg6 Sr2 3.7268(16) 2_656 ?
Mg6 Sr6 3.7484(15) 1_455 ?
Mg6 Sr1 3.9143(16) 2_656 ?
F1 Mg5 1.928(3) 2_545 ?
F1 Sr5 2.691(2) 2_645 ?
F1 Sr6 2.896(3) 2_646 ?
F2 Mg6 1.967(3) 2_546 ?
F2 Sr5 2.607(2) 2_646 ?
F2 Sr6 2.758(3) 2_646 ?
F3 Sr6 2.495(3) 2_646 ?
F3 Sr5 2.534(3) 2_645 ?
F4 Sr6 2.538(3) 2_646 ?
F4 Sr5 2.562(3) 2_646 ?
F5 Mg6 1.911(3) 2_646 ?
F6 Sr6 2.716(3) 2_646 ?
F7 Mg1 2.016(3) 1_556 ?
F7 Sr5 2.569(3) 2_646 ?
F8 Sr4 2.531(3) 1_554 ?
F11 Sr1 2.524(3) 1_556 ?
F12 Mg2 1.931(3) 1_655 ?
F13 Mg1 1.933(3) 1_656 ?
F13 Sr1 3.055(3) 1_556 ?
F14 Mg4 1.953(3) 1_454 ?
F14 Sr4 2.742(3) 1_554 ?
F15 Mg3 1.947(3) 1_455 ?
F16 Mg4 1.966(3) 1_554 ?
F17 Sr4 3.187(3) 1_655 ?
F18 Sr4 2.508(3) 1_554 ?
F21 Sr5 2.386(3) 1_556 ?
F22 Sr2 3.127(3) 2_656 ?
F23 Mg5 1.992(3) 1_556 ?
F23 Sr6 2.844(2) 1_455 ?
F24 Sr1 2.439(3) 2_655 ?
F24 Sr2 2.523(3) 2_656 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F5 Sr1 F24 100.61(10) . 2_645 ?
F5 Sr1 F3 71.51(8) . . ?
F24 Sr1 F3 71.60(9) 2_645 . ?
F5 Sr1 F10 73.87(9) . . ?
F24 Sr1 F10 170.84(9) 2_645 . ?
F3 Sr1 F10 99.51(8) . . ?
F5 Sr1 F16 115.30(9) . . ?
F24 Sr1 F16 123.41(9) 2_645 . ?
F3 Sr1 F16 159.01(8) . . ?
F10 Sr1 F16 65.74(9) . . ?
F5 Sr1 F11 177.36(9) . 1_554 ?
F24 Sr1 F11 76.79(8) 2_645 1_554 ?
F3 Sr1 F11 107.00(8) . 1_554 ?
F10 Sr1 F11 108.64(9) . 1_554 ?
F16 Sr1 F11 66.88(8) . 1_554 ?
F5 Sr1 F8 112.28(8) . . ?
F24 Sr1 F8 110.56(8) 2_645 . ?
F3 Sr1 F8 64.57(8) . . ?
F10 Sr1 F8 66.07(8) . . ?
F16 Sr1 F8 95.01(9) . . ?
F11 Sr1 F8 68.53(8) 1_554 . ?
F5 Sr1 F13 125.36(8) . 1_554 ?
F24 Sr1 F13 64.67(8) 2_645 1_554 ?
F3 Sr1 F13 135.09(8) . 1_554 ?
F10 Sr1 F13 124.46(8) . 1_554 ?
F16 Sr1 F13 59.00(8) . 1_554 ?
F11 Sr1 F13 54.07(7) 1_554 1_554 ?
F8 Sr1 F13 122.24(7) . 1_554 ?
F5 Sr1 F12 57.46(8) . . ?
F24 Sr1 F12 132.04(8) 2_645 . ?
F3 Sr1 F12 125.55(8) . . ?
F10 Sr1 F12 51.28(7) . . ?
F16 Sr1 F12 57.86(7) . . ?
F11 Sr1 F12 124.65(7) 1_554 . ?
F8 Sr1 F12 117.18(7) . . ?
F13 Sr1 F12 92.53(6) 1_554 . ?
F5 Sr1 Mg4 145.14(7) . 1_554 ?
F24 Sr1 Mg4 92.37(7) 2_645 1_554 ?
F3 Sr1 Mg4 143.24(7) . 1_554 ?
F10 Sr1 Mg4 96.25(7) . 1_554 ?
F16 Sr1 Mg4 35.03(6) . 1_554 ?
F11 Sr1 Mg4 36.25(6) 1_554 1_554 ?
F8 Sr1 Mg4 92.60(6) . 1_554 ?
F13 Sr1 Mg4 35.71(5) 1_554 1_554 ?
F12 Sr1 Mg4 89.97(5) . 1_554 ?
F5 Sr1 Mg3 86.13(7) . . ?
F24 Sr1 Mg3 153.54(7) 2_645 . ?
F3 Sr1 Mg3 134.24(7) . . ?
F10 Sr1 Mg3 34.95(6) . . ?
F16 Sr1 Mg3 34.57(7) . . ?
F11 Sr1 Mg3 96.41(7) 1_554 . ?
F8 Sr1 Mg3 89.84(6) . . ?
F13 Sr1 Mg3 90.46(5) 1_554 . ?
F12 Sr1 Mg3 34.59(5) . . ?
Mg4 Sr1 Mg3 69.28(3) 1_554 . ?
F5 Sr1 Mg1 95.12(6) . . ?
F24 Sr1 Mg1 87.75(6) 2_645 . ?
F3 Sr1 Mg1 32.27(6) . . ?
F10 Sr1 Mg1 85.51(6) . . ?
F16 Sr1 Mg1 127.76(7) . . ?
F11 Sr1 Mg1 84.36(6) 1_554 . ?
F8 Sr1 Mg1 32.79(6) . . ?
F13 Sr1 Mg1 133.22(5) 1_554 . ?
F12 Sr1 Mg1 132.08(5) . . ?
Mg4 Sr1 Mg1 117.77(4) 1_554 . ?
Mg3 Sr1 Mg1 117.35(4) . . ?
F5 Sr2 F4 73.03(8) . . ?
F5 Sr2 F10 73.19(8) . . ?
F4 Sr2 F10 96.34(8) . . ?
F5 Sr2 F24 112.58(10) . 2_646 ?
F4 Sr2 F24 72.55(9) . 2_646 ?
F10 Sr2 F24 164.30(9) . 2_646 ?
F5 Sr2 F11 167.79(9) . . ?
F4 Sr2 F11 101.52(8) . . ?
F10 Sr2 F11 96.98(9) . . ?
F24 Sr2 F11 75.09(8) 2_646 . ?
F5 Sr2 F13 130.50(9) . . ?
F4 Sr2 F13 142.52(9) . . ?
F10 Sr2 F13 117.10(8) . . ?
F24 Sr2 F13 71.13(8) 2_646 . ?
F11 Sr2 F13 60.20(8) . . ?
F5 Sr2 F12 66.84(8) . . ?
F4 Sr2 F12 137.80(9) . . ?
F10 Sr2 F12 60.37(8) . . ?
F24 Sr2 F12 135.21(8) 2_646 . ?
F11 Sr2 F12 115.07(8) . . ?
F13 Sr2 F12 77.32(8) . . ?
F5 Sr2 F9 106.23(8) . . ?
F4 Sr2 F9 60.82(8) . . ?
F10 Sr2 F9 59.81(8) . . ?
F24 Sr2 F9 104.59(7) 2_646 . ?
F11 Sr2 F9 61.91(8) . . ?
F13 Sr2 F9 120.90(8) . . ?
F12 Sr2 F9 118.83(8) . . ?
F5 Sr2 F17 117.98(8) . . ?
F4 Sr2 F17 145.60(8) . . ?
F10 Sr2 F17 60.68(8) . . ?
F24 Sr2 F17 123.22(8) 2_646 . ?
F11 Sr2 F17 60.51(8) . . ?
F13 Sr2 F17 57.16(8) . . ?
F12 Sr2 F17 55.40(8) . . ?
F9 Sr2 F17 84.91(7) . . ?
F5 Sr2 F22 57.83(8) . 2_646 ?
F4 Sr2 F22 69.83(8) . 2_646 ?
F10 Sr2 F22 131.00(8) . 2_646 ?
F24 Sr2 F22 56.43(8) 2_646 2_646 ?
F11 Sr2 F22 131.33(8) . 2_646 ?
F13 Sr2 F22 97.02(8) . 2_646 ?
F12 Sr2 F22 98.19(8) . 2_646 ?
F9 Sr2 F22 130.63(8) . 2_646 ?
F17 Sr2 F22 144.45(7) . 2_646 ?
F5 Sr2 Mg3 84.44(7) . . ?
F4 Sr2 Mg3 130.50(7) . . ?
F10 Sr2 Mg3 34.31(6) . . ?
F24 Sr2 Mg3 155.95(6) 2_646 . ?
F11 Sr2 Mg3 91.38(7) . . ?
F13 Sr2 Mg3 84.92(6) . . ?
F12 Sr2 Mg3 34.88(6) . . ?
F9 Sr2 Mg3 85.53(6) . . ?
F17 Sr2 Mg3 34.69(6) . . ?
F22 Sr2 Mg3 131.60(6) 2_646 . ?
F5 Sr2 Mg4 149.29(7) . . ?
F4 Sr2 Mg4 136.50(7) . . ?
F10 Sr2 Mg4 91.95(7) . . ?
F24 Sr2 Mg4 89.01(7) 2_646 . ?
F11 Sr2 Mg4 34.99(6) . . ?
F13 Sr2 Mg4 34.90(6) . . ?
F12 Sr2 Mg4 82.45(6) . . ?
F9 Sr2 Mg4 87.90(6) . . ?
F17 Sr2 Mg4 34.66(6) . . ?
F22 Sr2 Mg4 131.00(6) 2_646 . ?
Mg3 Sr2 Mg4 69.32(3) . . ?
F9 Sr3 F10 67.18(8) . . ?
F9 Sr3 F8 94.86(10) . . ?
F10 Sr3 F8 69.03(8) . . ?
F9 Sr3 F22 128.26(9) . . ?
F10 Sr3 F22 147.37(9) . . ?
F8 Sr3 F22 128.13(9) . . ?
F9 Sr3 F18 166.43(9) . . ?
F10 Sr3 F18 101.22(8) . . ?
F8 Sr3 F18 73.74(9) . . ?
F22 Sr3 F18 65.31(8) . . ?
F9 Sr3 F19 76.02(9) . . ?
F10 Sr3 F19 98.25(8) . . ?
F8 Sr3 F19 166.71(8) . . ?
F22 Sr3 F19 64.77(8) . . ?
F18 Sr3 F19 113.81(9) . . ?
F9 Sr3 F14 125.32(8) . . ?
F10 Sr3 F14 134.29(8) . . ?
F8 Sr3 F14 66.29(8) . . ?
F22 Sr3 F14 65.30(8) . . ?
F18 Sr3 F14 57.31(8) . . ?
F19 Sr3 F14 126.87(8) . . ?
F9 Sr3 F20 111.62(8) . . ?
F10 Sr3 F20 62.71(9) . . ?
F8 Sr3 F20 106.82(8) . . ?
F22 Sr3 F20 84.81(9) . . ?
F18 Sr3 F20 66.19(8) . . ?
F19 Sr3 F20 68.73(8) . . ?
F14 Sr3 F20 122.83(8) . . ?
F9 Sr3 F15 67.21(8) . . ?
F10 Sr3 F15 132.65(8) . . ?
F8 Sr3 F15 126.98(8) . . ?
F22 Sr3 F15 64.05(8) . . ?
F18 Sr3 F15 125.49(8) . . ?
F19 Sr3 F15 58.69(7) . . ?
F14 Sr3 F15 83.92(8) . . ?
F20 Sr3 F15 126.20(8) . . ?
F9 Sr3 Mg5 154.10(6) . . ?
F10 Sr3 Mg5 138.19(7) . . ?
F8 Sr3 Mg5 92.13(7) . . ?
F22 Sr3 Mg5 36.43(7) . . ?
F18 Sr3 Mg5 36.97(6) . . ?
F19 Sr3 Mg5 100.26(6) . . ?
F14 Sr3 Mg5 37.85(6) . . ?
F20 Sr3 Mg5 89.99(6) . . ?
F15 Sr3 Mg5 88.75(6) . . ?
F9 Sr3 Mg6 92.35(7) . . ?
F10 Sr3 Mg6 135.46(7) . . ?
F8 Sr3 Mg6 154.97(6) . . ?
F22 Sr3 Mg6 36.49(7) . . ?
F18 Sr3 Mg6 101.07(7) . . ?
F19 Sr3 Mg6 37.27(6) . . ?
F14 Sr3 Mg6 90.07(6) . . ?
F20 Sr3 Mg6 92.61(6) . . ?
F15 Sr3 Mg6 36.95(6) . . ?
Mg5 Sr3 Mg6 71.81(4) . . ?
F9 Sr3 Mg3 88.86(6) . . ?
F10 Sr3 Mg3 30.87(6) . . ?
F8 Sr3 Mg3 87.55(6) . . ?
F22 Sr3 Mg3 116.58(7) . . ?
F18 Sr3 Mg3 83.41(6) . . ?
F19 Sr3 Mg3 82.69(6) . . ?
F14 Sr3 Mg3 136.87(6) . . ?
F20 Sr3 Mg3 31.84(6) . . ?
F15 Sr3 Mg3 137.81(6) . . ?
Mg5 Sr3 Mg3 116.37(4) . . ?
Mg6 Sr3 Mg3 116.57(4) . . ?
F9 Sr4 F11 69.27(8) . . ?
F9 Sr4 F18 154.31(8) . 1_556 ?
F11 Sr4 F18 90.66(8) . 1_556 ?
F9 Sr4 F8 112.25(9) . 1_556 ?
F11 Sr4 F8 70.81(8) . 1_556 ?
F18 Sr4 F8 73.57(9) 1_556 1_556 ?
F9 Sr4 F19 76.01(9) . . ?
F11 Sr4 F19 88.48(8) . . ?
F18 Sr4 F19 88.00(9) 1_556 . ?
F8 Sr4 F19 151.67(8) 1_556 . ?
F9 Sr4 F15 65.60(8) . . ?
F11 Sr4 F15 128.56(8) . . ?
F18 Sr4 F15 122.18(8) 1_556 . ?
F8 Sr4 F15 150.31(8) 1_556 . ?
F19 Sr4 F15 58.02(7) . . ?
F9 Sr4 F14 149.18(8) . 1_556 ?
F11 Sr4 F14 129.68(8) . 1_556 ?
F18 Sr4 F14 56.44(8) 1_556 1_556 ?
F8 Sr4 F14 64.20(8) 1_556 1_556 ?
F19 Sr4 F14 122.70(8) . 1_556 ?
F15 Sr4 F14 101.75(8) . 1_556 ?
F9 Sr4 F23 123.15(8) . . ?
F11 Sr4 F23 142.88(8) . . ?
F18 Sr4 F23 64.46(8) 1_556 . ?
F8 Sr4 F23 121.96(8) 1_556 . ?
F19 Sr4 F23 64.86(8) . . ?
F15 Sr4 F23 59.11(7) . . ?
F14 Sr4 F23 59.67(7) 1_556 . ?
F9 Sr4 F7 58.94(8) . . ?
F11 Sr4 F7 72.41(8) . . ?
F18 Sr4 F7 131.46(8) 1_556 . ?
F8 Sr4 F7 57.96(8) 1_556 . ?
F19 Sr4 F7 134.71(8) . . ?
F15 Sr4 F7 102.86(7) . . ?
F14 Sr4 F7 100.26(7) 1_556 . ?
F23 Sr4 F7 144.71(7) . . ?
F9 Sr4 F17 97.51(8) . 1_455 ?
F11 Sr4 F17 155.98(8) . 1_455 ?
F18 Sr4 F17 106.63(8) 1_556 1_455 ?
F8 Sr4 F17 97.74(8) 1_556 1_455 ?
F19 Sr4 F17 108.23(7) . 1_455 ?
F15 Sr4 F17 55.11(7) . 1_455 ?
F14 Sr4 F17 55.07(7) 1_556 1_455 ?
F23 Sr4 F17 61.13(8) . 1_455 ?
F7 Sr4 F17 83.61(7) . 1_455 ?
F9 Sr4 Mg6 89.65(7) . . ?
F11 Sr4 Mg6 124.33(7) . . ?
F18 Sr4 Mg6 88.84(7) 1_556 . ?
F8 Sr4 Mg6 157.58(7) 1_556 . ?
F19 Sr4 Mg6 35.86(6) . . ?
F15 Sr4 Mg6 35.79(6) . . ?
F14 Sr4 Mg6 94.63(6) 1_556 . ?
F23 Sr4 Mg6 35.73(6) . . ?
F7 Sr4 Mg6 138.46(6) . . ?
F17 Sr4 Mg6 73.68(6) 1_455 . ?
F9 Sr4 Mg5 158.53(7) . 1_556 ?
F11 Sr4 Mg5 125.67(7) . 1_556 ?
F18 Sr4 Mg5 35.02(6) 1_556 1_556 ?
F8 Sr4 Mg5 88.51(7) 1_556 1_556 ?
F19 Sr4 Mg5 88.28(6) . 1_556 ?
F15 Sr4 Mg5 93.75(6) . 1_556 ?
F14 Sr4 Mg5 36.28(6) 1_556 1_556 ?
F23 Sr4 Mg5 35.42(6) . 1_556 ?
F7 Sr4 Mg5 136.30(6) . 1_556 ?
F17 Sr4 Mg5 73.33(6) 1_455 1_556 ?
Mg6 Sr4 Mg5 69.27(4) . 1_556 ?
F21 Sr5 F18 69.19(9) 1_554 . ?
F21 Sr5 F20 97.63(10) 1_554 . ?
F18 Sr5 F20 70.03(8) . . ?
F21 Sr5 F3 72.67(9) 1_554 2_655 ?
F18 Sr5 F3 96.74(9) . 2_655 ?
F20 Sr5 F3 166.02(9) . 2_655 ?
F21 Sr5 F4 169.89(9) 1_554 2_656 ?
F18 Sr5 F4 103.09(8) . 2_656 ?
F20 Sr5 F4 73.15(9) . 2_656 ?
F3 Sr5 F4 115.59(9) 2_655 2_656 ?
F21 Sr5 F7 125.04(9) 1_554 2_656 ?
F18 Sr5 F7 145.63(9) . 2_656 ?
F20 Sr5 F7 129.06(9) . 2_656 ?
F3 Sr5 F7 64.57(8) 2_655 2_656 ?
F4 Sr5 F7 65.03(8) 2_656 2_656 ?
F21 Sr5 F2 122.24(8) 1_554 2_656 ?
F18 Sr5 F2 137.76(8) . 2_656 ?
F20 Sr5 F2 68.17(8) . 2_656 ?
F3 Sr5 F2 125.39(8) 2_655 2_656 ?
F4 Sr5 F2 58.81(8) 2_656 2_656 ?
F7 Sr5 F2 65.92(8) 2_656 2_656 ?
F21 Sr5 F24 111.89(8) 1_554 . ?
F18 Sr5 F24 64.31(9) . . ?
F20 Sr5 F24 109.35(8) . . ?
F3 Sr5 F24 66.78(8) 2_655 . ?
F4 Sr5 F24 68.57(8) 2_656 . ?
F7 Sr5 F24 81.51(8) 2_656 . ?
F2 Sr5 F24 125.77(8) 2_656 . ?
F21 Sr5 F1 65.66(8) 1_554 2_655 ?
F18 Sr5 F1 133.22(9) . 2_655 ?
F20 Sr5 F1 127.09(8) . 2_655 ?
F3 Sr5 F1 58.77(8) 2_655 2_655 ?
F4 Sr5 F1 123.09(8) 2_656 2_655 ?
F7 Sr5 F1 63.29(8) 2_656 2_655 ?
F2 Sr5 F1 79.41(8) 2_656 2_655 ?
F24 Sr5 F1 123.54(8) . 2_655 ?
F21 Sr5 Mg2 150.32(7) 1_554 2_656 ?
F18 Sr5 Mg2 140.16(7) . 2_656 ?
F20 Sr5 Mg2 91.87(7) . 2_656 ?
F3 Sr5 Mg2 101.49(6) 2_655 2_656 ?
F4 Sr5 Mg2 37.08(6) 2_656 2_656 ?
F7 Sr5 Mg2 37.29(6) 2_656 2_656 ?
F2 Sr5 Mg2 37.74(6) 2_656 2_656 ?
F24 Sr5 Mg2 90.99(6) . 2_656 ?
F1 Sr5 Mg2 86.19(6) 2_655 2_656 ?
F21 Sr5 Mg1 88.47(7) 1_554 2_655 ?
F18 Sr5 Mg1 133.25(7) . 2_655 ?
F20 Sr5 Mg1 156.07(7) . 2_655 ?
F3 Sr5 Mg1 36.55(6) 2_655 2_655 ?
F4 Sr5 Mg1 101.64(6) 2_656 2_655 ?
F7 Sr5 Mg1 37.03(6) 2_656 2_655 ?
F2 Sr5 Mg1 88.97(6) 2_656 2_655 ?
F24 Sr5 Mg1 89.42(6) . 2_655 ?
F1 Sr5 Mg1 36.43(6) 2_655 2_655 ?
Mg2 Sr5 Mg1 72.53(4) 2_656 2_655 ?
F21 Sr5 Mg5 93.12(7) 1_554 . ?
F18 Sr5 Mg5 31.88(6) . . ?
F20 Sr5 Mg5 86.30(6) . . ?
F3 Sr5 Mg5 84.26(6) 2_655 . ?
F4 Sr5 Mg5 82.32(6) 2_656 . ?
F7 Sr5 Mg5 114.31(6) 2_656 . ?
F2 Sr5 Mg5 137.76(6) 2_656 . ?
F24 Sr5 Mg5 32.86(6) . . ?
F1 Sr5 Mg5 140.90(6) 2_655 . ?
Mg2 Sr5 Mg5 115.59(4) 2_656 . ?
Mg1 Sr5 Mg5 116.58(4) 2_655 . ?
F21 Sr6 F3 72.78(9) . 2_656 ?
F21 Sr6 F20 115.30(10) . . ?
F3 Sr6 F20 150.05(9) 2_656 . ?
F21 Sr6 F4 153.28(9) . 2_656 ?
F3 Sr6 F4 87.82(9) 2_656 2_656 ?
F20 Sr6 F4 73.42(9) . 2_656 ?
F21 Sr6 F19 70.65(8) . . ?
F3 Sr6 F19 85.94(8) 2_656 . ?
F20 Sr6 F19 71.33(8) . . ?
F4 Sr6 F19 90.22(8) 2_656 . ?
F21 Sr6 F6 119.10(9) . 2_656 ?
F3 Sr6 F6 63.84(8) 2_656 2_656 ?
F20 Sr6 F6 123.85(8) . 2_656 ?
F4 Sr6 F6 64.59(8) 2_656 2_656 ?
F19 Sr6 F6 140.05(8) . 2_656 ?
F21 Sr6 F17 62.32(9) . . ?
F3 Sr6 F17 135.01(9) 2_656 . ?
F20 Sr6 F17 62.29(9) . . ?
F4 Sr6 F17 135.21(8) 2_656 . ?
F19 Sr6 F17 82.22(8) . . ?
F6 Sr6 F17 137.59(8) 2_656 . ?
F21 Sr6 F2 149.46(8) . 2_656 ?
F3 Sr6 F2 122.95(8) 2_656 2_656 ?
F20 Sr6 F2 65.66(8) . 2_656 ?
F4 Sr6 F2 57.10(7) 2_656 2_656 ?
F19 Sr6 F2 131.43(8) . 2_656 ?
F6 Sr6 F2 60.78(7) 2_656 2_656 ?
F17 Sr6 F2 96.52(8) . 2_656 ?
F21 Sr6 F23 89.92(8) . 1_655 ?
F3 Sr6 F23 113.03(8) 2_656 1_655 ?
F20 Sr6 F23 96.20(8) . 1_655 ?
F4 Sr6 F23 114.98(8) 2_656 1_655 ?
F19 Sr6 F23 148.00(8) . 1_655 ?
F6 Sr6 F23 71.52(7) 2_656 1_655 ?
F17 Sr6 F23 66.07(8) . 1_655 ?
F2 Sr6 F23 60.32(7) 2_656 1_655 ?
F21 Sr6 F1 61.89(8) . 2_656 ?
F3 Sr6 F1 56.28(8) 2_656 2_656 ?
F20 Sr6 F1 153.64(8) . 2_656 ?
F4 Sr6 F1 121.88(8) 2_656 2_656 ?
F19 Sr6 F1 125.44(8) . 2_656 ?
F6 Sr6 F1 58.96(7) 2_656 2_656 ?
F17 Sr6 F1 97.49(8) . 2_656 ?
F2 Sr6 F1 102.96(7) 2_656 2_656 ?
F23 Sr6 F1 58.53(7) 1_655 2_656 ?
F21 Sr6 Mg2 154.34(7) . 2_656 ?
F3 Sr6 Mg2 88.00(7) 2_656 2_656 ?
F20 Sr6 Mg2 89.86(7) . 2_656 ?
F4 Sr6 Mg2 35.85(6) 2_656 2_656 ?
F19 Sr6 Mg2 125.95(6) . 2_656 ?
F6 Sr6 Mg2 35.28(6) 2_656 2_656 ?
F17 Sr6 Mg2 133.17(6) . 2_656 ?
F2 Sr6 Mg2 36.70(5) 2_656 2_656 ?
F23 Sr6 Mg2 81.98(6) 1_655 2_656 ?
F1 Sr6 Mg2 93.44(6) 2_656 2_656 ?
F21 Sr6 Mg1 86.02(7) . 2_656 ?
F3 Sr6 Mg1 35.18(6) 2_656 2_656 ?
F20 Sr6 Mg1 158.57(7) . 2_656 ?
F4 Sr6 Mg1 88.43(6) 2_656 2_656 ?
F19 Sr6 Mg1 121.12(6) . 2_656 ?
F6 Sr6 Mg1 35.10(6) 2_656 2_656 ?
F17 Sr6 Mg1 132.85(7) . 2_656 ?
F2 Sr6 Mg1 95.09(6) 2_656 2_656 ?
F23 Sr6 Mg1 80.96(6) 1_655 2_656 ?
F1 Sr6 Mg1 35.37(5) 2_656 2_656 ?
Mg2 Sr6 Mg1 68.72(3) 2_656 2_656 ?
F13 Mg1 F6 94.81(12) 1_454 . ?
F13 Mg1 F8 96.88(13) 1_454 . ?
F6 Mg1 F8 98.27(12) . . ?
F13 Mg1 F1 95.36(12) 1_454 . ?
F6 Mg1 F1 88.69(12) . . ?
F8 Mg1 F1 165.34(13) . . ?
F13 Mg1 F3 174.67(14) 1_454 . ?
F6 Mg1 F3 88.17(12) . . ?
F8 Mg1 F3 87.05(11) . . ?
F1 Mg1 F3 80.26(12) . . ?
F13 Mg1 F7 91.22(12) 1_454 1_554 ?
F6 Mg1 F7 173.03(14) . 1_554 ?
F8 Mg1 F7 84.44(12) . 1_554 ?
F1 Mg1 F7 87.27(12) . 1_554 ?
F3 Mg1 F7 85.55(12) . 1_554 ?
F13 Mg1 Sr5 125.75(10) 1_454 2_645 ?
F6 Mg1 Sr5 123.05(10) . 2_645 ?
F8 Mg1 Sr5 112.19(9) . 2_645 ?
F1 Mg1 Sr5 53.59(8) . 2_645 ?
F3 Mg1 Sr5 49.07(8) . 2_645 ?
F7 Mg1 Sr5 50.12(8) 1_554 2_645 ?
F13 Mg1 Sr6 133.63(10) 1_454 2_646 ?
F6 Mg1 Sr6 52.38(8) . 2_646 ?
F8 Mg1 Sr6 117.33(9) . 2_646 ?
F1 Mg1 Sr6 57.60(8) . 2_646 ?
F3 Mg1 Sr6 46.03(8) . 2_646 ?
F7 Mg1 Sr6 120.68(10) 1_554 2_646 ?
Sr5 Mg1 Sr6 70.83(3) 2_645 2_646 ?
F13 Mg1 Sr1 142.05(10) 1_454 . ?
F6 Mg1 Sr1 100.30(9) . . ?
F8 Mg1 Sr1 46.74(8) . . ?
F1 Mg1 Sr1 119.42(9) . . ?
F3 Mg1 Sr1 41.03(8) . . ?
F7 Mg1 Sr1 76.84(8) 1_554 . ?
Sr5 Mg1 Sr1 72.72(3) 2_645 . ?
Sr6 Mg1 Sr1 81.63(3) 2_646 . ?
F13 Mg1 Mg4 21.34(8) 1_454 1_454 ?
F6 Mg1 Mg4 89.81(9) . 1_454 ?
F8 Mg1 Mg4 77.09(9) . 1_454 ?
F1 Mg1 Mg4 116.03(9) . 1_454 ?
F3 Mg1 Mg4 163.54(10) . 1_454 ?
F7 Mg1 Mg4 97.07(10) 1_554 1_454 ?
Sr5 Mg1 Mg4 142.01(5) 2_645 1_454 ?
Sr6 Mg1 Mg4 139.67(5) 2_646 1_454 ?
Sr1 Mg1 Mg4 123.69(5) . 1_454 ?
F13 Mg1 Sr4 73.57(9) 1_454 1_554 ?
F6 Mg1 Sr4 132.14(10) . 1_554 ?
F8 Mg1 Sr4 40.66(8) . 1_554 ?
F1 Mg1 Sr4 137.63(10) . 1_554 ?
F3 Mg1 Sr4 107.61(9) . 1_554 ?
F7 Mg1 Sr4 53.20(9) 1_554 1_554 ?
Sr5 Mg1 Sr4 99.57(4) 2_645 1_554 ?
Sr6 Mg1 Sr4 152.08(4) 2_646 1_554 ?
Sr1 Mg1 Sr4 70.46(3) . 1_554 ?
Mg4 Mg1 Sr4 62.57(3) 1_454 1_554 ?
F13 Mg1 Sr3 86.44(9) 1_454 . ?
F6 Mg1 Sr3 71.06(8) . . ?
F8 Mg1 Sr3 30.13(8) . . ?
F1 Mg1 Sr3 159.76(9) . . ?
F3 Mg1 Sr3 98.72(9) . . ?
F7 Mg1 Sr3 112.89(9) 1_554 . ?
Sr5 Mg1 Sr3 138.75(4) 2_645 . ?
Sr6 Mg1 Sr3 107.30(4) 2_646 . ?
Sr1 Mg1 Sr3 66.39(3) . . ?
Mg4 Mg1 Sr3 65.25(3) 1_454 . ?
Sr4 Mg1 Sr3 62.15(2) 1_554 . ?
F12 Mg2 F9 91.65(12) 1_455 . ?
F12 Mg2 F6 96.03(12) 1_455 . ?
F9 Mg2 F6 97.77(12) . . ?
F12 Mg2 F4 173.93(14) 1_455 . ?
F9 Mg2 F4 88.46(12) . . ?
F6 Mg2 F4 89.97(12) . . ?
F12 Mg2 F7 87.44(12) 1_455 . ?
F9 Mg2 F7 86.01(12) . . ?
F6 Mg2 F7 174.77(14) . . ?
F4 Mg2 F7 86.52(12) . . ?
F12 Mg2 F2 101.52(11) 1_455 . ?
F9 Mg2 F2 165.28(13) . . ?
F6 Mg2 F2 87.47(11) . . ?
F4 Mg2 F2 77.75(11) . . ?
F7 Mg2 F2 88.01(12) . . ?
F12 Mg2 Sr5 124.58(9) 1_455 2_646 ?
F9 Mg2 Sr5 115.13(10) . 2_646 ?
F6 Mg2 Sr5 124.33(10) . 2_646 ?
F4 Mg2 Sr5 50.31(8) . 2_646 ?
F7 Mg2 Sr5 50.50(8) . 2_646 ?
F2 Mg2 Sr5 51.59(8) . 2_646 ?
F12 Mg2 Sr6 136.43(10) 1_455 2_646 ?
F9 Mg2 Sr6 119.19(10) . 2_646 ?
F6 Mg2 Sr6 52.82(8) . 2_646 ?
F4 Mg2 Sr6 47.76(8) . 2_646 ?
F7 Mg2 Sr6 122.12(10) . 2_646 ?
F2 Mg2 Sr6 54.03(8) . 2_646 ?
Sr5 Mg2 Sr6 71.79(3) 2_646 2_646 ?
F12 Mg2 Sr4 69.30(9) 1_455 . ?
F9 Mg2 Sr4 39.85(8) . . ?
F6 Mg2 Sr4 130.98(10) . . ?
F4 Mg2 Sr4 107.34(9) . . ?
F7 Mg2 Sr4 53.98(8) . . ?
F2 Mg2 Sr4 140.30(9) . . ?
Sr5 Mg2 Sr4 100.56(4) 2_646 . ?
Sr6 Mg2 Sr4 153.31(4) 2_646 . ?
F12 Mg2 Mg3 19.80(8) 1_455 1_455 ?
F9 Mg2 Mg3 74.58(9) . 1_455 ?
F6 Mg2 Mg3 88.42(9) . 1_455 ?
F4 Mg2 Mg3 162.57(10) . 1_455 ?
F7 Mg2 Mg3 96.09(9) . 1_455 ?
F2 Mg2 Mg3 119.50(9) . 1_455 ?
Sr5 Mg2 Mg3 141.38(5) 2_646 1_455 ?
Sr6 Mg2 Mg3 138.77(5) 2_646 1_455 ?
Sr4 Mg2 Mg3 61.78(3) . 1_455 ?
F12 Mg2 Mg6 82.49(9) 1_455 2_546 ?
F9 Mg2 Mg6 172.50(10) . 2_546 ?
F6 Mg2 Mg6 78.29(9) . 2_546 ?
F4 Mg2 Mg6 97.87(9) . 2_546 ?
F7 Mg2 Mg6 98.35(9) . 2_546 ?
F2 Mg2 Mg6 22.11(7) . 2_546 ?
Sr5 Mg2 Mg6 72.23(4) 2_646 2_546 ?
Sr6 Mg2 Mg6 63.52(3) 2_646 2_546 ?
Sr4 Mg2 Mg6 139.90(5) . 2_546 ?
Mg3 Mg2 Mg6 98.80(4) 1_455 2_546 ?
F12 Mg2 Sr2 141.03(10) 1_455 . ?
F9 Mg2 Sr2 51.58(8) . . ?
F6 Mg2 Sr2 100.90(9) . . ?
F4 Mg2 Sr2 37.60(8) . . ?
F7 Mg2 Sr2 78.59(8) . . ?
F2 Mg2 Sr2 113.98(8) . . ?
Sr5 Mg2 Sr2 71.97(3) 2_646 . ?
Sr6 Mg2 Sr2 80.23(3) 2_646 . ?
Sr4 Mg2 Sr2 73.11(3) . . ?
Mg3 Mg2 Sr2 126.03(5) 1_455 . ?
Mg6 Mg2 Sr2 135.17(5) 2_546 . ?
F15 Mg3 F16 91.22(12) 1_655 . ?
F15 Mg3 F20 98.16(12) 1_655 . ?
F16 Mg3 F20 94.60(13) . . ?
F15 Mg3 F10 176.06(14) 1_655 . ?
F16 Mg3 F10 86.06(12) . . ?
F20 Mg3 F10 84.91(12) . . ?
F15 Mg3 F12 96.87(12) 1_655 . ?
F16 Mg3 F12 91.85(12) . . ?
F20 Mg3 F12 163.50(14) . . ?
F10 Mg3 F12 80.39(12) . . ?
F15 Mg3 F17 89.60(12) 1_655 . ?
F16 Mg3 F17 177.90(13) . . ?
F20 Mg3 F17 87.20(13) . . ?
F10 Mg3 F17 93.02(12) . . ?
F12 Mg3 F17 86.13(12) . . ?
F15 Mg3 Sr1 130.52(10) 1_655 . ?
F16 Mg3 Sr1 45.77(8) . . ?
F20 Mg3 Sr1 107.00(10) . . ?
F10 Mg3 Sr1 45.81(8) . . ?
F12 Mg3 Sr1 67.45(9) . . ?
F17 Mg3 Sr1 132.58(10) . . ?
F15 Mg3 Sr2 135.21(10) 1_655 . ?
F16 Mg3 Sr2 114.50(10) . . ?
F20 Mg3 Sr2 114.45(10) . . ?
F10 Mg3 Sr2 44.33(8) . . ?
F12 Mg3 Sr2 49.18(8) . . ?
F17 Mg3 Sr2 63.66(9) . . ?
Sr1 Mg3 Sr2 69.36(3) . . ?
F15 Mg3 Sr6 81.01(9) 1_655 . ?
F16 Mg3 Sr6 132.58(10) . . ?
F20 Mg3 Sr6 41.70(8) . . ?
F10 Mg3 Sr6 102.93(10) . . ?
F12 Mg3 Sr6 135.41(10) . . ?
F17 Mg3 Sr6 49.48(9) . . ?
Sr1 Mg3 Sr6 143.32(5) . . ?
Sr2 Mg3 Sr6 102.98(4) . . ?
F15 Mg3 Sr3 143.43(10) 1_655 . ?
F16 Mg3 Sr3 90.42(9) . . ?
F20 Mg3 Sr3 45.31(8) . . ?
F10 Mg3 Sr3 39.60(8) . . ?
F12 Mg3 Sr3 119.59(9) . . ?
F17 Mg3 Sr3 90.07(9) . . ?
Sr1 Mg3 Sr3 72.11(3) . . ?
Sr2 Mg3 Sr3 75.63(3) . . ?
Sr6 Mg3 Sr3 71.27(3) . . ?
F15 Mg3 Mg2 80.16(9) 1_655 1_655 ?
F16 Mg3 Mg2 82.72(9) . 1_655 ?
F20 Mg3 Mg2 176.77(11) . 1_655 ?
F10 Mg3 Mg2 96.65(10) . 1_655 ?
F12 Mg3 Mg2 19.27(8) . 1_655 ?
F17 Mg3 Mg2 95.52(10) . 1_655 ?
Sr1 Mg3 Mg2 72.39(4) . 1_655 ?
Sr2 Mg3 Mg2 68.43(4) . 1_655 ?
Sr6 Mg3 Mg2 140.07(5) . 1_655 ?
Sr3 Mg3 Mg2 136.21(5) . 1_655 ?
F15 Mg3 Sr4 44.44(8) 1_655 1_655 ?
F16 Mg3 Sr4 121.80(10) . 1_655 ?
F20 Mg3 Sr4 122.00(10) . 1_655 ?
F10 Mg3 Sr4 135.47(10) . 1_655 ?
F12 Mg3 Sr4 66.02(9) . 1_655 ?
F17 Mg3 Sr4 57.82(9) . 1_655 ?
Sr1 Mg3 Sr4 130.93(5) . 1_655 ?
Sr2 Mg3 Sr4 91.15(4) . 1_655 ?
Sr6 Mg3 Sr4 83.62(3) . 1_655 ?
Sr3 Mg3 Sr4 147.70(5) . 1_655 ?
Mg2 Mg3 Sr4 58.54(3) 1_655 1_655 ?
F21 Mg4 F14 91.73(13) . 1_656 ?
F21 Mg4 F16 95.86(13) . 1_556 ?
F14 Mg4 F16 90.31(12) 1_656 1_556 ?
F21 Mg4 F17 87.40(13) . . ?
F14 Mg4 F17 89.17(13) 1_656 . ?
F16 Mg4 F17 176.71(15) 1_556 . ?
F21 Mg4 F13 170.37(14) . . ?
F14 Mg4 F13 96.77(11) 1_656 . ?
F16 Mg4 F13 88.64(12) 1_556 . ?
F17 Mg4 F13 88.19(12) . . ?
F21 Mg4 F11 91.68(12) . . ?
F14 Mg4 F11 176.23(14) 1_656 . ?
F16 Mg4 F11 87.75(12) 1_556 . ?
F17 Mg4 F11 92.59(13) . . ?
F13 Mg4 F11 79.97(12) . . ?
F21 Mg4 Sr1 114.54(10) . 1_556 ?
F14 Mg4 Sr1 128.97(10) 1_656 1_556 ?
F16 Mg4 Sr1 46.44(8) 1_556 1_556 ?
F17 Mg4 Sr1 132.30(11) . 1_556 ?
F13 Mg4 Sr1 63.03(8) . 1_556 ?
F11 Mg4 Sr1 47.82(8) . 1_556 ?
F21 Mg4 Sr2 122.26(10) . . ?
F14 Mg4 Sr2 132.36(10) 1_656 . ?
F16 Mg4 Sr2 115.19(10) 1_556 . ?
F17 Mg4 Sr2 63.08(9) . . ?
F13 Mg4 Sr2 48.20(8) . . ?
F11 Mg4 Sr2 46.24(8) . . ?
Sr1 Mg4 Sr2 69.53(3) 1_556 . ?
F21 Mg4 Sr6 38.87(9) . . ?
F14 Mg4 Sr6 82.89(9) 1_656 . ?
F16 Mg4 Sr6 133.44(10) 1_556 . ?
F17 Mg4 Sr6 49.69(9) . . ?
F13 Mg4 Sr6 137.85(10) . . ?
F11 Mg4 Sr6 100.78(9) . . ?
Sr1 Mg4 Sr6 144.21(5) 1_556 . ?
Sr2 Mg4 Sr6 102.66(4) . . ?
F21 Mg4 Mg1 168.88(11) . 1_656 ?
F14 Mg4 Mg1 77.46(9) 1_656 1_656 ?
F16 Mg4 Mg1 81.77(10) 1_556 1_656 ?
F17 Mg4 Mg1 94.94(10) . 1_656 ?
F13 Mg4 Mg1 20.58(7) . 1_656 ?
F11 Mg4 Mg1 99.06(9) . 1_656 ?
Sr1 Mg4 Mg1 71.58(4) 1_556 1_656 ?
Sr2 Mg4 Mg1 68.14(4) . 1_656 ?
Sr6 Mg4 Mg1 139.78(5) . 1_656 ?
F21 Mg4 Mg5 69.89(9) . 1_656 ?
F14 Mg4 Mg5 22.64(8) 1_656 1_656 ?
F16 Mg4 Mg5 98.19(10) 1_556 1_656 ?
F17 Mg4 Mg5 82.51(10) . 1_656 ?
F13 Mg4 Mg5 117.96(9) . 1_656 ?
F11 Mg4 Mg5 161.05(10) . 1_656 ?
Sr1 Mg4 Mg5 143.75(6) 1_556 1_656 ?
Sr2 Mg4 Mg5 141.18(5) . 1_656 ?
Sr6 Mg4 Mg5 62.21(3) . 1_656 ?
Mg1 Mg4 Mg5 99.59(5) 1_656 1_656 ?
F21 Mg4 Sr4 114.63(10) . 1_655 ?
F14 Mg4 Sr4 43.22(8) 1_656 1_655 ?
F16 Mg4 Sr4 121.34(10) 1_556 1_655 ?
F17 Mg4 Sr4 56.54(9) . 1_655 ?
F13 Mg4 Sr4 69.56(8) . 1_655 ?
F11 Mg4 Sr4 135.99(10) . 1_655 ?
Sr1 Mg4 Sr4 130.34(4) 1_556 1_655 ?
Sr2 Mg4 Sr4 89.93(4) . 1_655 ?
Sr6 Mg4 Sr4 82.97(3) . 1_655 ?
Mg1 Mg4 Sr4 58.78(3) 1_656 1_655 ?
Mg5 Mg4 Sr4 54.44(3) 1_656 1_655 ?
F1 Mg5 F22 90.71(12) 2 . ?
F1 Mg5 F24 94.79(12) 2 . ?
F22 Mg5 F24 86.85(12) . . ?
F1 Mg5 F23 91.43(12) 2 1_554 ?
F22 Mg5 F23 174.49(14) . 1_554 ?
F24 Mg5 F23 98.03(12) . 1_554 ?
F1 Mg5 F18 177.48(14) 2 . ?
F22 Mg5 F18 87.31(12) . . ?
F24 Mg5 F18 86.65(12) . . ?
F23 Mg5 F18 90.41(12) 1_554 . ?
F1 Mg5 F14 102.03(11) 2 . ?
F22 Mg5 F14 88.50(12) . . ?
F24 Mg5 F14 162.59(12) . . ?
F23 Mg5 F14 86.09(12) 1_554 . ?
F18 Mg5 F14 76.38(12) . . ?
F1 Mg5 Sr3 127.40(10) 2 . ?
F22 Mg5 Sr3 49.65(8) . . ?
F24 Mg5 Sr3 112.52(9) . . ?
F23 Mg5 Sr3 125.48(10) 1_554 . ?
F18 Mg5 Sr3 50.08(9) . . ?
F14 Mg5 Sr3 53.00(8) . . ?
F1 Mg5 Sr4 134.33(10) 2 1_554 ?
F22 Mg5 Sr4 121.44(10) . 1_554 ?
F24 Mg5 Sr4 116.62(9) . 1_554 ?
F23 Mg5 Sr4 53.99(8) 1_554 1_554 ?
F18 Mg5 Sr4 46.16(8) . 1_554 ?
F14 Mg5 Sr4 52.94(8) . 1_554 ?
Sr3 Mg5 Sr4 71.87(3) . 1_554 ?
F1 Mg5 Sr5 140.40(10) 2 . ?
F22 Mg5 Sr5 80.14(9) . . ?
F24 Mg5 Sr5 46.63(8) . . ?
F23 Mg5 Sr5 101.33(9) 1_554 . ?
F18 Mg5 Sr5 40.65(8) . . ?
F14 Mg5 Sr5 116.00(9) . . ?
Sr3 Mg5 Sr5 73.66(3) . . ?
Sr4 Mg5 Sr5 81.00(3) 1_554 . ?
F1 Mg5 Mg4 81.70(9) 2 1_454 ?
F22 Mg5 Mg4 96.25(10) . 1_454 ?
F24 Mg5 Mg4 175.32(10) . 1_454 ?
F23 Mg5 Mg4 79.04(9) 1_554 1_454 ?
F18 Mg5 Mg4 96.97(10) . 1_454 ?
F14 Mg5 Mg4 21.69(7) . 1_454 ?
Sr3 Mg5 Mg4 72.14(4) . 1_454 ?
Sr4 Mg5 Mg4 64.64(4) 1_554 1_454 ?
Sr5 Mg5 Mg4 137.32(5) . 1_454 ?
F1 Mg5 Sr6 49.17(8) 2 1_454 ?
F22 Mg5 Sr6 131.56(9) . 1_454 ?
F24 Mg5 Sr6 117.79(9) . 1_454 ?
F23 Mg5 Sr6 47.95(8) 1_554 1_454 ?
F18 Mg5 Sr6 131.74(9) . 1_454 ?
F14 Mg5 Sr6 77.42(8) . 1_454 ?
Sr3 Mg5 Sr6 129.70(4) . 1_454 ?
Sr4 Mg5 Sr6 85.86(4) 1_554 1_454 ?
Sr5 Mg5 Sr6 147.45(5) . 1_454 ?
Mg4 Mg5 Sr6 57.55(3) 1_454 1_454 ?
F1 Mg5 Sr2 74.44(9) 2 2_656 ?
F22 Mg5 Sr2 56.01(9) . 2_656 ?
F24 Mg5 Sr2 38.17(8) . 2_656 ?
F23 Mg5 Sr2 129.50(10) 1_554 2_656 ?
F18 Mg5 Sr2 105.64(9) . 2_656 ?
F14 Mg5 Sr2 143.84(10) . 2_656 ?
Sr3 Mg5 Sr2 99.85(4) . 2_656 ?
Sr4 Mg5 Sr2 149.45(5) 1_554 2_656 ?
Sr5 Mg5 Sr2 68.49(3) . 2_656 ?
Mg4 Mg5 Sr2 142.27(5) 1_454 2_656 ?
Sr6 Mg5 Sr2 119.27(4) 1_454 2_656 ?
F5 Mg6 F2 90.73(12) 2_656 2_556 ?
F5 Mg6 F22 89.96(13) 2_656 . ?
F2 Mg6 F22 92.25(12) 2_556 . ?
F5 Mg6 F23 96.91(13) 2_656 . ?
F2 Mg6 F23 90.33(12) 2_556 . ?
F22 Mg6 F23 172.63(14) . . ?
F5 Mg6 F15 173.30(13) 2_656 . ?
F2 Mg6 F15 95.48(11) 2_556 . ?
F22 Mg6 F15 87.29(12) . . ?
F23 Mg6 F15 85.59(12) . . ?
F5 Mg6 F19 94.44(12) 2_656 . ?
F2 Mg6 F19 174.55(14) 2_556 . ?
F22 Mg6 F19 86.04(12) . . ?
F23 Mg6 F19 90.76(12) . . ?
F15 Mg6 F19 79.28(12) . . ?
F5 Mg6 Sr3 121.03(10) 2_656 . ?
F2 Mg6 Sr3 124.91(10) 2_556 . ?
F22 Mg6 Sr3 49.18(8) . . ?
F23 Mg6 Sr3 124.12(10) . . ?
F15 Mg6 Sr3 52.97(8) . . ?
F19 Mg6 Sr3 50.52(8) . . ?
F5 Mg6 Sr4 123.93(10) 2_656 . ?
F2 Mg6 Sr4 129.93(10) 2_556 . ?
F22 Mg6 Sr4 119.45(10) . . ?
F23 Mg6 Sr4 54.18(8) . . ?
F15 Mg6 Sr4 52.99(8) . . ?
F19 Mg6 Sr4 47.60(8) . . ?
Sr3 Mg6 Sr4 70.32(3) . . ?
F5 Mg6 Mg2 68.58(9) 2_656 2_556 ?
F2 Mg6 Mg2 22.93(8) 2_556 2_556 ?
F22 Mg6 Mg2 97.72(10) . 2_556 ?
F23 Mg6 Mg2 87.31(9) . 2_556 ?
F15 Mg6 Mg2 117.85(9) . 2_556 ?
F19 Mg6 Mg2 162.50(10) . 2_556 ?
Sr3 Mg6 Mg2 141.84(6) . 2_556 ?
Sr4 Mg6 Mg2 138.92(5) . 2_556 ?
F5 Mg6 Sr2 35.58(9) 2_656 2_656 ?
F2 Mg6 Sr2 79.91(9) 2_556 2_656 ?
F22 Mg6 Sr2 57.02(9) . 2_656 ?
F23 Mg6 Sr2 130.29(10) . 2_656 ?
F15 Mg6 Sr2 143.49(10) . 2_656 ?
F19 Mg6 Sr2 103.37(9) . 2_656 ?
Sr3 Mg6 Sr2 100.27(4) . 2_656 ?
Sr4 Mg6 Sr2 149.26(5) . 2_656 ?
Mg2 Mg6 Sr2 65.51(3) 2_556 2_656 ?
F5 Mg6 Sr6 109.90(10) 2_656 1_455 ?
F2 Mg6 Sr6 45.62(8) 2_556 1_455 ?
F22 Mg6 Sr6 131.31(10) . 1_455 ?
F23 Mg6 Sr6 48.36(8) . 1_455 ?
F15 Mg6 Sr6 76.39(8) . 1_455 ?
F19 Mg6 Sr6 133.27(10) . 1_455 ?
Sr3 Mg6 Sr6 128.82(4) . 1_455 ?
Sr4 Mg6 Sr6 86.20(3) . 1_455 ?
Mg2 Mg6 Sr6 54.45(3) 2_556 1_455 ?
Sr2 Mg6 Sr6 119.80(4) 2_656 1_455 ?
F5 Mg6 Sr1 27.03(9) 2_656 2_656 ?
F2 Mg6 Sr1 89.27(9) 2_556 2_656 ?
F22 Mg6 Sr1 116.99(10) . 2_656 ?
F23 Mg6 Sr1 69.93(9) . 2_656 ?
F15 Mg6 Sr1 155.11(10) . 2_656 ?
F19 Mg6 Sr1 96.13(9) . 2_656 ?
Sr3 Mg6 Sr1 139.46(4) . 2_656 ?
Sr4 Mg6 Sr1 106.15(4) . 2_656 ?
Mg2 Mg6 Sr1 66.90(3) 2_556 2_656 ?
Sr2 Mg6 Sr1 61.40(3) 2_656 2_656 ?
Sr6 Mg6 Sr1 89.95(3) 1_455 2_656 ?
Mg5 F1 Mg1 142.68(15) 2_545 . ?
Mg5 F1 Sr5 126.28(12) 2_545 2_645 ?
Mg1 F1 Sr5 89.97(9) . 2_645 ?
Mg5 F1 Sr6 100.59(11) 2_545 2_646 ?
Mg1 F1 Sr6 87.03(9) . 2_646 ?
Sr5 F1 Sr6 89.13(7) 2_645 2_646 ?
Mg6 F2 Mg2 134.95(14) 2_546 . ?
Mg6 F2 Sr5 129.82(12) 2_546 2_646 ?
Mg2 F2 Sr5 90.67(9) . 2_646 ?
Mg6 F2 Sr6 103.72(11) 2_546 2_646 ?
Mg2 F2 Sr6 89.27(9) . 2_646 ?
Sr5 F2 Sr6 94.75(8) 2_646 2_646 ?
Mg1 F3 Sr1 106.70(11) . . ?
Mg1 F3 Sr6 98.79(11) . 2_646 ?
Sr1 F3 Sr6 135.52(11) . 2_646 ?
Mg1 F3 Sr5 94.37(11) . 2_645 ?
Sr1 F3 Sr5 110.95(10) . 2_645 ?
Sr6 F3 Sr5 102.56(9) 2_646 2_645 ?
Mg2 F4 Sr2 112.46(12) . . ?
Mg2 F4 Sr6 96.39(10) . 2_646 ?
Sr2 F4 Sr6 134.04(11) . 2_646 ?
Mg2 F4 Sr5 92.61(10) . 2_646 ?
Sr2 F4 Sr5 111.64(10) . 2_646 ?
Sr6 F4 Sr5 101.45(9) 2_646 2_646 ?
Mg6 F5 Sr1 131.52(14) 2_646 . ?
Mg6 F5 Sr2 117.31(13) 2_646 . ?
Sr1 F5 Sr2 108.31(11) . . ?
Mg2 F6 Mg1 156.21(15) . . ?
Mg2 F6 Sr6 91.90(10) . 2_646 ?
Mg1 F6 Sr6 92.52(10) . 2_646 ?
Mg1 F7 Mg2 156.07(15) 1_556 . ?
Mg1 F7 Sr5 92.85(11) 1_556 2_646 ?
Mg2 F7 Sr5 92.20(11) . 2_646 ?
Mg1 F7 Sr4 93.63(10) 1_556 . ?
Mg2 F7 Sr4 92.46(10) . . ?
Sr5 F7 Sr4 152.85(10) 2_646 . ?
Mg1 F8 Sr3 126.37(12) . . ?
Mg1 F8 Sr4 108.81(12) . 1_554 ?
Sr3 F8 Sr4 104.42(10) . 1_554 ?
Mg1 F8 Sr1 100.47(12) . . ?
Sr3 F8 Sr1 107.97(9) . . ?
Sr4 F8 Sr1 107.77(9) 1_554 . ?
Mg2 F9 Sr3 129.10(13) . . ?
Mg2 F9 Sr4 110.01(12) . . ?
Sr3 F9 Sr4 104.14(10) . . ?
Mg2 F9 Sr2 97.09(11) . . ?
Sr3 F9 Sr2 107.24(8) . . ?
Sr4 F9 Sr2 107.72(9) . . ?
Mg3 F10 Sr2 101.37(11) . . ?
Mg3 F10 Sr3 109.53(12) . . ?
Sr2 F10 Sr3 124.23(11) . . ?
Mg3 F10 Sr1 99.24(11) . . ?
Sr2 F10 Sr1 104.52(10) . . ?
Sr3 F10 Sr1 114.46(10) . . ?
Mg4 F11 Sr4 122.46(13) . . ?
Mg4 F11 Sr1 95.93(10) . 1_556 ?
Sr4 F11 Sr1 112.88(10) . 1_556 ?
Mg4 F11 Sr2 98.77(11) . . ?
Sr4 F11 Sr2 120.97(10) . . ?
Sr1 F11 Sr2 101.24(9) 1_556 . ?
Mg2 F12 Mg3 140.94(15) 1_655 . ?
Mg2 F12 Sr2 123.07(12) 1_655 . ?
Mg3 F12 Sr2 95.94(10) . . ?
Mg2 F12 Sr1 106.39(11) 1_655 . ?
Mg3 F12 Sr1 77.96(9) . . ?
Sr2 F12 Sr1 83.10(7) . . ?
Mg1 F13 Mg4 138.08(15) 1_656 . ?
Mg1 F13 Sr2 123.20(12) 1_656 . ?
Mg4 F13 Sr2 96.90(10) . . ?
Mg1 F13 Sr1 109.99(11) 1_656 1_556 ?
Mg4 F13 Sr1 81.26(9) . 1_556 ?
Sr2 F13 Sr1 87.03(7) . 1_556 ?
Mg4 F14 Mg5 135.66(14) 1_454 . ?
Mg4 F14 Sr3 127.48(12) 1_454 . ?
Mg5 F14 Sr3 89.16(9) . . ?
Mg4 F14 Sr4 107.59(11) 1_454 1_554 ?
Mg5 F14 Sr4 90.78(9) . 1_554 ?
Sr3 F14 Sr4 94.66(7) . 1_554 ?
Mg3 F15 Mg6 139.12(14) 1_455 . ?
Mg3 F15 Sr3 125.11(12) 1_455 . ?
Mg6 F15 Sr3 90.08(9) . . ?
Mg3 F15 Sr4 105.70(12) 1_455 . ?
Mg6 F15 Sr4 91.22(9) . . ?
Sr3 F15 Sr4 92.31(7) . . ?
Mg3 F16 Mg4 159.16(17) . 1_554 ?
Mg3 F16 Sr1 99.66(11) . . ?
Mg4 F16 Sr1 98.53(11) 1_554 . ?
Mg3 F17 Mg4 163.60(17) . . ?
Mg3 F17 Sr6 97.36(12) . . ?
Mg4 F17 Sr6 96.87(12) . . ?
Mg3 F17 Sr2 81.65(10) . . ?
Mg4 F17 Sr2 82.26(10) . . ?
Sr6 F17 Sr2 139.22(10) . . ?
Mg3 F17 Sr4 90.40(10) . 1_655 ?
Mg4 F17 Sr4 92.03(11) . 1_655 ?
Sr6 F17 Sr4 111.18(9) . 1_655 ?
Sr2 F17 Sr4 109.60(8) . 1_655 ?
Mg5 F18 Sr5 107.47(12) . . ?
Mg5 F18 Sr4 98.82(10) . 1_554 ?
Sr5 F18 Sr4 133.97(11) . 1_554 ?
Mg5 F18 Sr3 92.95(10) . . ?
Sr5 F18 Sr3 112.11(10) . . ?
Sr4 F18 Sr3 103.31(10) 1_554 . ?
Mg6 F19 Sr4 96.54(10) . . ?
Mg6 F19 Sr6 121.42(13) . . ?
Sr4 F19 Sr6 129.72(10) . . ?
Mg6 F19 Sr3 92.22(10) . . ?
Sr4 F19 Sr3 98.97(9) . . ?
Sr6 F19 Sr3 110.08(9) . . ?
Mg3 F20 Sr5 124.70(13) . . ?
Mg3 F20 Sr6 106.64(12) . . ?
Sr5 F20 Sr6 104.74(10) . . ?
Mg3 F20 Sr3 102.85(12) . . ?
Sr5 F20 Sr3 107.69(9) . . ?
Sr6 F20 Sr3 109.81(9) . . ?
Mg4 F21 Sr5 131.69(14) . 1_556 ?
Mg4 F21 Sr6 111.50(13) . . ?
Sr5 F21 Sr6 109.42(11) 1_556 . ?
Mg5 F22 Mg6 159.68(16) . . ?
Mg5 F22 Sr3 93.92(11) . . ?
Mg6 F22 Sr3 94.33(11) . . ?
Mg5 F22 Sr2 92.45(10) . 2_656 ?
Mg6 F22 Sr2 90.72(10) . 2_656 ?
Sr3 F22 Sr2 146.91(11) . 2_656 ?
Mg5 F23 Mg6 155.32(16) 1_556 . ?
Mg5 F23 Sr4 90.60(10) 1_556 . ?
Mg6 F23 Sr4 90.08(10) . . ?
Mg5 F23 Sr6 100.71(10) 1_556 1_455 ?
Mg6 F23 Sr6 99.89(10) . 1_455 ?
Sr4 F23 Sr6 121.61(9) . 1_455 ?
Mg5 F24 Sr1 124.80(13) . 2_655 ?
Mg5 F24 Sr2 112.68(12) . 2_656 ?
Sr1 F24 Sr2 104.03(10) 2_655 2_656 ?
Mg5 F24 Sr5 100.50(11) . . ?
Sr1 F24 Sr5 107.23(9) 2_655 . ?
Sr2 F24 Sr5 106.23(9) 2_656 . ?

_diffrn_measured_fraction_theta_max 0.999
_diffrn_reflns_theta_full        28.28
_diffrn_measured_fraction_theta_full 0.999
_refine_diff_density_max         0.765
_refine_diff_density_min         -0.730
_refine_diff_density_rms         0.133
_database_code_depnum_ccdc_archive 'CCDC 1029322'
